Spreadsheet: 1403920c-df9b-4d7c-b276-2e2a4318bbf5
Sheet: Sheet1

Tolerances on shape and dimesions for cold rolled products according to EN 485-4 | Unnamed: 1 | Unnamed: 2 | Unnamed: 3 | Unnamed: 4 | Unnamed: 5 | Unnamed: 6 | Unnamed: 7 | Unnamed: 8 | Unnamed: 9
 | Thickness tolerances for sheet, strip and plate
 | Specified thickness t |  | Thickness tolerance for specified [NAME]
 |  |  | w≤1000 | 1000<w≤1250 | 1000<w≤1250 | 1000<w≤1250 | 1000<w≤1250 | 1000<w≤1250 | 1000<w≤1250
 | t > | t ≤ | Alloy Group | Alloy Group | Alloy Group | Alloy Group | Alloy Group | Alloy Group | Alloy Group
 |  |  | I          II | I          II | I          II | I          II | I          II | I          II | I          II
 | 0,20 | 0,4 | ± 0,02  ± 0,03 | ± 0,04  ± 0,05 | ± 0,05  ± 0,06 | -           - | - | - | -
 | 0,4 | 0,5 | ± 0,03  ± 0,03 | ± 0,04  ± 0,05 | ± 0,05  ± 0,06 | ± 0,06  ± 0,07 | ± 0,10 | - | -
 | 0,5 | 0,6 | ± 0,03  ± 0,04 | ± 0,05  ± 0,06 | ± 0,06  ± 0,07 | ± 0,07  ± 0,08 | ± 0,11 | - | -
 | 0,6 | 0,8 | ± 0,03  ± 0,04 | ± 0,06  ± 0,07 | ± 0,07  ± 0,08 | ± 0,08  ± 0,09 | ± 0,12 | - | -
 | 0,8 | 1,0 | ± 0,04  ± 0,05 | ± 0,06  ± 0,08 | ± 0,08  ± 0,09 | ± 0,09  ± 0,10 | ± 0,13 | - | -
 | 1,0 | 1,2 | ± 0,04  ± 0,05 | ± 0,07  ± 0,09 | ± 0,09  ± 0,10 | ± 0,10  ± 0,12 | ± 0,14 | - | -
 | 1,2 | 1,5 | ± 0,05  ± 0,07 | ± 0,09  ± 0,11 | ± 0,10  ± 0,12 | ± 0,11  ± 0,14 | ± 0,16 | - | -
 | 1,5 | 1,8 | ± 0,06  ± 0,08 | ± 0,10  ± 0,12 | ± 0,11  ± 0,13 | ± 0,12  ± 0,15 | ± 0,17 | - | -
 | 1,8 | 2 | ± 0,06  ± 0,09 | ± 0,11  ± 0,13 | ± 0,12  ± 0,14 | ± 0,14  ± 0,16 | ± 0,19 | - | -
 | 2 | 2,5 | ± 0,07  ± 0,10 | ± 0,12  ± 0,14 | ± 0,13  ± 0,15 | ± 0,15  ± 0,17 | ± 0,20 | - | -
 | 2,5 | 3,0 | ± 0,08  ± 0,11 | ± 0,13  ± 0,15 | ± 0,15  ± 0,17 | ± 0,17  ± 0,19 | ± 0,23 | - | -
 | 3,0 | 3,5 | ± 0,10  ± 0,12 | ± 0,15  ± 0,17 | ± 0,17  ± 0,19 | ± 0,18  ± 0,20 | ± 0,24 | - | -
 | 3,5 | 4,0 | ± 0,15 | ± 0,20 | ± 0,22 | ± 0,23 | ± 0,25 | ± 0,34 | ± 0,38
 | 4,0 | 5,0 | ± 0,18 | ± 0,22 | ± 0,24 | ± 0,25 | ± 0,29 | ± 0,36 | ± 0,42
 | 5,0 | 6,0 | ± 0,20 | ± 0,24 | ± 0,25 | ± 0,26 | ± 0,32 | ± 0,40 | ± 0,46
 | 6,0 | 8,0 | ± 0,24 | ± 0,30 | ± 0,31 | ± 0,32 | ± 0,38 | ± 0,44 | ± 0,50
 | 8,0 | 10,0 | ± 0,27 | ± 0,33 | ± 0,36 | ± 0,38 | ± 0,44 | ± 0,50 | ± 0,56
 | 10 | 12 | ± 0,32 | ± 0,38 | ± 0,40 | ± 0,41 | ± 0,47 | ± 0,53 | ± 0,59
 | 12 | 15 | ± 0,36 | ± 0,42 | ± 0,43 | ± 0,45 | ± 0,51 | ± 0,57 | ± 0,63
 | 15 | 20 | ± 0,38 | ± 0,44 | ± 0,46 | ± 0,48 | ± 0,54 | ± 0,60 | ± 0,66
 | When measuring the thickness, a zone 10 [NAME] wide from the edges of th product shall be disregarded
 | Group I alloys : |  | 1000-series alloys, non heat-treatable 7000 and 8000 series alloys
 |  |  | 4000 series alloys with less than 2% maximum specified silicon content
 |  |  | 3000 and 5000 series alloys, for which the maximum specified magnesium and manganese contents
 |  |  |  | are each no greater than 1,8% and their sum no greater than 2,3%
 | Group II alloys : |  | All alloys which do not belong to Group I
 | [NAME] tolerances for strip
 | Specified thickness |  | [NAME] tolerance for specified [NAME]
 | t > | t ≤ | [NAME] 100 | 100<w≤300 | 100<w≤300 | 100<w≤300 | 100<w≤300 | 100<w≤300
 | 0,20 | 0,6 | 0 / +0,3 | 0 / +0,4 | 0 / +0,6 | 0 / +1,5 | 0 / +2,5 | 0 / +3
 | 0,6 | 1,0 | 0 / +0,3 | 0 / +0,5 | 0 / +1 | 0 / +1,5 | 0 / +2,5 | 0 / +3
 | 1,0 | 2,0 | 0 / +0,4 | 0 / +0,7 | 0 / +1,2 | 0 / +2 | 0 / +2,5 | 0 / +3
 | 2,0 | 3,0 | 0 / +1 | 0 / +1 | 0 / +1,5 | 0 / +2 | 0 / +2,5 | 0 / +4
 | 3,0 | 5,0 | - | 0 / +1,5 | 0 / +2 | 0 / +3 | 0 / +3 | 0 / +5
 | [NAME] tolerances for sheet and plate
 | Specified thickness t |  | [NAME] tolerance for specified [NAME]
 | t > | t ≤ | [NAME] 500 | 500<w≤1250 | 1250<w≤2000 | 2000<w≤3000 | 3000<w≤3500
 | 0,20 | 3,0 | 0 / +1,5 | 0 / +3 | 0 / +4 | 0 / +5 | -
 | 3,0 | 6,0 | 0 / +3 | 0 / +4 | 0 / +5 | 0 / +8 | 0 / +8
 | 6,0 | 50 | 0 / +4 | 0 / +5 | 0 / +5 | 0 / +8 | 0 / +8
 | Length tolerances for sheet and plate
 | Specified thickness t |  | Length tolerance for specified length L
 | t > | t ≤ | L ≤ 500 | 1000<L≤2000 | 2000<L≤3000 | 3000<L≤5000 | Over 5000
 | 0,20 | 3,0 | 0 / +3 | 0 / +4 | 0 / +6 | 0 / +8 | + 0,2 %
 | 3,0 | 6,0 | 0 / +4 | 0 / +6 | 0 / +8 | 0 / +10 | of specified length
 | 6,0 | 50 | 0 / +6 | 0 / +8 | 0 / +10 | 0 / +10
 | Lateral curvature tolerances for strip
 | (measured on 2000 mm strip length)
 | Specified width w |  | Lateral curvature
 | w > | [NAME] | dmax
 | ≥25 | 100 | 8
 | 100 | 300 | 6
 | 300 | 600 | 5
 | 600 | 1000 | 4
 | 1000 | 2000 | 3
 | 2000 | 3500 | 3
 | For widths less than 25 mm the tolerance are to be
 | agreed between purchaser and supplier
 | Lateral curvature tolerances for sheet and plate
 | Specified width w |  | Lateral curvature dmax for specified length L
 | w > | [NAME] | [NAME] | 1000<w≤2000 | 2000<w≤3500 | 3500<w≤5000 | 5000<w≤15000
 | ≥100 | 300 | 2 | 4 | 8 | - | -
 | 300 | 600 | 1,5 | 3 | 5 | - | -
 | 600 | 1000 | 1 | 2 | 4 | 5 | + 0,1 %
 | 1000 | 2000 | - | 2 | 4 | 5 | of specified length
 | 2000 | 3500 | - | - | 4 | 5
 | for widths less than 100 mm the tolerance are to be agreed between purchaser and supplier
 | Flatness tolerance for sheet and plate
 | Specified thickness t |  | Total deviation |  |  |  | Partial deviation %
 | t > | t ≤ | on length |  | on width |  | (for a chord ≥ 300 mm)
 |  |  | dmax / L |  | dmax / w |  | dmax / L
 | 0,20 | 0,50 | by agreement |  | by agreement |  | by agreement
 | 0,50 | 3,0 | 0,5 |  | 0,5 |  | 0,5
 | 3,0 | 6,0 | 0,4 |  | 0,4 |  | 0,4
 | 6,0 | 50 | 0,4 |  | 0,3 |  | 0,3
 | Squareness tolerances for sheet and plate
 | Specified length L |  | Specified thickness t | Squareness tolerance for specified [NAME]
 | L > | L ≤ |  | [NAME] | 1000<w≤1500 | 1500<w≤2000 | 2000<w≤3500
 |  | 1000 | ≤ 6 | 4 | - | - | -
 |  |  | > 6 | 5 | - | - | -
 | 1000 | 2000 | ≤ 6 | 4 | 5 | 6 | -
 |  |  | > 6 | 6 | 7 | 8 | -
 | 2000 | 3000 | ≤ 6 | 5 | 5 | 7 | 8
 |  |  | > 6 | 7 | 7 | 9 | 10
 | 3000 | 5000 | ≤ 6 | 6 | 8 | 8 | 10
 |  |  | > 6 | 8 | 10 | 10 | 12
 | 5000 | 15000 | ≤ 6 | 10 | 10 | 12 | 12
 |  |  | > 6 | 12 | 12 | 15 | 15